Silver nanoparticle incorporation effect on mechanical and thermal properties of denture base acrylic resins $\úHJO.g52ö/812QXUù$+ø11,úÕQ.h5.dh2ö/82'R÷XgPU'('(37RQJXog='(0ø54, Baki HAZER5 %OHQW(FHYLW8QLYHUVLW\)DFXOW\RI'HQWLVWU\'HSDUWPHQWRI3URVWKRGRQWLFV=RQJXOGDN7XUNH\ 6OH\PDQ'HPLUHO8QLYHUVLW\)DFXOW\RI'HQWLVWU\'HSDUWPHQWRI3URVWKRGRQWLFV,VSDUWD7XUNH\ 3- Ordu University, Faculty of Dentistry, Department of Prosthodontics, Ordu, Turkey. 4- Mersin University, Faculty of Engineering, Department of Chemical Engineering, Mersin, Turkey. %OHQW(FHYLW8QLYHUVLW\)DFXOW\RI$UWVDQG6FLHQFHV'HSDUWPHQWRI&KHPLVWU\=RQJXOGDN7XUNH\ Corresponding address:2QXUùDKLQ%OHQW(FHYLW8QLYHUVLW\)DFXOW\RI'HQWLVWU\'HSDUWPHQWRI3URVWKRGRQWLFV=RQJXOGDN7XUNH\3RVWFRGH - Phone: +903722613536 - Fax: +903722613403 - e-mail: [email protected]
bjective: The aim of the present study was to evaluate the mechanical and thermal characteristics of two denture base acrylic resins containing silver nanoparticles (AgNPs). Material and Methods: Two different acrylic denture base resins (heat-polymerized and microwave polymerized) containing 0.3, 0.8 and 1.6 wt% AgNPs were evaluated for ÀH[XUDOVWUHQJWKHODVWLFPRGXOXVDQGLPSDFWVWUHQJWK7KHJODVVWUDQVLWLRQWHPSHUDWXUH (Tg) and relative heat capacity (Cp) of the samples were determined from the Differential Scanning Calorimetry (DSC) results. For statistical analysis, two-way ANOVA and TukeyHSD tests were performed. Results: Addition of 0.8% and 1.6% AgNPs in microwaveSRO\PHUL]HGUHVLQVLJQL¿FDQWO\GHFUHDVHGWKHWUDQVYHUVHVWUHQJWKDQGHODVWLFPRGXOXV,Q terms of impact strength, the addition of AgNPs has no effect on both resin groups. Glass transition temperature (Tg) was decreased with the addition of AgNPs for both denture base resins. Conclusions: The incorporation of AgNPs, generally used for antimicrobial HI¿FLHQF\DIIHFWHGWKHWUDQVYHUVHVWUHQJWKRIWKHGHQWXUHEDVHDFU\OLFUHVLQVGHSHQGLQJ on the concentration of nanoparticles. Tg was decreased with the addition of AgNPs for both denture base resins. Keywords: Nanoparticles. Acrylic resin. Flexural strength. Impact strength. Differential scanning calorimetry.
broad-spectrum antimicrobial acrylic resin materials has attracted much interest in recent times13. Silver (Ag) salts have been used for thousands RI\HDUVEHFDXVHRIWKHLUDQWLPLFURELDOHI¿FLHQF\ against Gram-positive and Gram-negative bacteria, protozoa and fungi, as well as viruses18. Nowadays, elemental Ag and associated compounds are used to reduce the risk of infection in the treatment of burns, prevent bacterial colonization on medical devices, in VXUJLFDOWH[WLOHIDEULFVIRUZDWHUSXUL¿FDWLRQERQH cements, and dental materials11-14,18,24. In dental applications, different forms of Ag such as Ag ions (Ag+), Ag nanoparticles (AgNPs), and Ag-polymeric complexes have been used to improve DQWLEDFWHULDO HI¿FLHQF\7,16. The instability of Ag+,
Poly(methyl methacrylate) (PMMA) is widely used in the preparation of partial and total denture bases. The proliferation of certain pathogens such as Candida albicans and Streptococcus mutans is induced by the surface roughness of acrylic resins and local or systemic factors1,6,25. The improvement of oral hygiene is generally achieved by the use of antimicrobial mouthwashes and appropriate tooth-brushing methods along with the use of denture cleansing tablets and prophylactic systemic antibiotics. However, all these methods have limited success in reducing the effectiveness of these pathogens7,19. For these reasons, research on
J Appl Oral Sci.
Silver nanoparticle incorporation effect on mechanical and thermal properties of denture base acrylic resins
liquid ratios for heat-polymerized and microwavepolymerized resin were 35 g/14 mL and 100 g/43 mL, respectively. For the study groups to determine the effect of AgNPs, the suspension of AgNPs was mixed with each resin monomer in concentrations of 0.3, 0.8, and 1.6 wt% and sonicated for 15 min. Afterwards, the liquid component was mixed with the powder part, in accordance with the manufacturer’s instructions. The heat-polymerized specimens were cured in a water bath at 100°C for 30 min while the microwave-polymerized specimens were irradiated for 3 min at 600 W. Before GHÀDVNLQJDOOWKHVSHFLPHQVZHUHEHQFKFRROHG Test specimens were wet ground with silicone carbide grinding papers of 200, 400, and 600-grit sizes using an automatic polishing machine (Grin 329JULQGHUSROLVKHU0HWNRQ$ù%XUVD7XUNH\ %HIRUHWHVWLQJIRUIXOOVDWXUDWLRQWKHÀH[XUDOWHVW specimens were kept in distilled water at 37°C for 50±2 h, and impact test specimens were stored at 37°C for 2 weeks8,15.
however, restricts its practical implementation. The problem can be resolved by protecting the Ag+ with a polymeric matrix sheath. The major advantage of using AgNPs arises from their large ratio of surface area to volume. AgNPs exhibit more effective ion release and enhanced antimicrobial activity5. AgNPs are preferred for this reason, alongside additional functional assets such as their ductility, electrical and thermal conductivity7,17,22,25. Although the antimicrobial characteristic of AgNPs in acrylic resins has been previously illustrated1,13,19,23,27, there are few studies reporting WKHLQÀXHQFHRI13VRQWKHPHFKDQLFDOSURSHUWLHV of denture base resins10,13,25. Although the addition of AgNPs has antimicrobial advantages on acrylic resins, its effect on the mechanical properties of the resin should be examined25. Therefore, the aim of this in vitro study was to evaluate the HIIHFW RI $J13V RQ WKH ÀH[XUDO VWUHQJWK HODVWLF modulus, impact strength, and differential scanning calorimetry (DSC) properties of two distinct dental acrylic resins.
Flexural strength testing
MATERIAL AND METHODS
7KH ÀH[XUDO VWUHQJWK WHVW ZDV SHUIRUPHG E\ using a Lloyd universal testing machine (Lloyd Instruments, LRX, Fareham, UK) with a crosshead speed of 5 mm/min. Flexural strength (FS) was determined using the following formula; FS=3Fl/2bh2 where F is the maximum load applied (N), l is the distance between supports (span length=50 mm), b is the width of the specimen (10 mm) and h is the thickness of the specimen (2.5 mm). Elastic modulus (E) was calculated from the formula; EM=Fl3/4bh3d ZKHUHGPP LVWKHGHÀHFWLRQ
Two acrylic resins used in this study were; (1) conventional heat-polymerized PMMA resin (Meliodent, Bayer Dental, Berkshire, UK); and (2) microwave-polymerized PMMA resin (Acron MC, GC Dental, Tokyo, Japan).
Synthesis and characterization of AgNPs The AgNPs were prepared based on the Turkevich method26. Silver nitrate (AgNO3) was dissolved in water (208 mg AgNO3/100 mL H2O) and the solution was brought to a boil (at 100°C). After 2 min of boiling, an aqueous solution of sodium citrate (Na3C6H5O7) (49 mg sodium citrate/1.25 g H2O) was added. The formation of AgNPs was perceived from the emergence of a yellow colour in the previously colourless solution. The solution was boiled further for another 6 min and then allowed to cool. Ultraviolet (UV) visible absorption spectroscopy (T80+, PG Instruments, Leicester, UK) and Transmission electron microscopy (TEM) (Technai G2 Spirit BioTWIN, FEI, OR, USA) were used to characterize the formation of AgNPs. Also, a Zeta Sizer Instrument (Malvern Instruments Ltd., Malvern, UK) was used to determine the particle size. Distilled water was used as a dispersion media during the particle size-determination process.
Impact strength testing Impact strength test was performed using a Charpy-type impact tester (Coesfeld, Pendulum Impact Tester, Dortmund, Germany). Impact strength (IS) was calculated using the following formula; IS=E/wt where E is the energy required to break the specimen (J), w is the width (6 mm) and t is the thickness of the specimen (4 mm).
Thermal analysis Differential Scanning Calorimetry (DSC) was performed with a Perkin Elmer Pyris 1 instrument and the analyses were carried out within a temperature range of 30°C to 200°C at a heating/ cooling rate of 20°C/min; Nitrogen was used as an inert atmosphere. 6 mg of sample was used for the DSC analysis and they were placed in an aluminium pan. The glass transition temperature
Specimen preparation In total, 56 specimens (n=7) were prepared for ÀH[XUDODQGLPSDFWVWUHQJWKWHVWVZLWKGLPHQVLRQV of 65×10×2.5 mm and 50×6×4 mm, according to the ADA Specification No.12 and ISO/DIS 1567:1998 standards, respectively. The powder/
J Appl Oral Sci.
(Tg) was taken as the peak temperature of the glass transition region. Tg and relative heat capacity (Cp) of the samples (control samples and 1.6 wt% AgNPs incorporated into microwave and heat polymerized samples) were determined from the DSC tests.
Synthesis and characterization of AgNPs According to the UV visible absorption spectroscopy AgNPs have a UV absorption band with a peak centered around 431 nm (Figure 1). Shape and size distribution of the synthesized AgNPs were characterized by TEM study. The TEM image shown in Figure 2 was obtained by high contrast TEM [FEI Technai G2 Spirit Bio (TWIN)]. The TEM image showed that the nano particles have rather similar and mainly spherical-like shapes.
Statistical analysis In each group, the mean and standard deviation values were calculated. For statistical analysis, twoway ANOVA and Tukey-HSD tests were performed. 6WDWLVWLFDOVLJQL¿FDQFHZDVVHWDWp